A molecular sieve is a material with pores (very small holes) of uniform size. These pore diameters are similar in size to small molecules, and thus large molecules cannot enter or be absorbed, while smaller molecules can. As a mixture of molecules migrate through the stationary bed of porous, semi-solid substance referred to as a sieve (or matrix), the components of highest molecular weight (which are unable to pass into the molecular pores) leave the bed first, followed by successively smaller molecules. Some molecular sieves are used in chromatography, a separation technique that sorts molecules based on their size. Other molecular sieves are used as desiccants (some examples include activated charcoal and silica gel).
The diameter of a molecular sieve is measured in ångströms (Å) or nanometres (nm). According to IUPAC notation, microporous materials have pore diameters of less than 2 nm (20 Å) and macroporous materials have pore diameters of greater than 50 nm (500 Å); the mesoporous category thus lies in the middle with pore diameters between 2 and 50 nm (20–500 Å).
- 1 Materials
- 2 Applications
- 3 Regeneration
- 4 Adsorption capabilities
- 5 3Å
- 6 4Å
- 7 5Å
- 8 See also
- 9 References
- 10 External links
Microporous material (<2 nm)
- Zeolites (aluminosilicate minerals, not to be confused with aluminium silicate)
- Zeolite LTA: 3–4 Å
- Porous glass: 10 Å (1 nm), and up
- Active carbon: 0–20 Å (0–2 nm), and up
- Montmorillonite intermixes
- Halloysite (endellite): Two common forms are found, when hydrated the clay exhibits a 1 nm spacing of the layers and when dehydrated (meta-halloysite) the spacing is 0.7 nm. Halloysite naturally occurs as small cylinders which average 30 nm in diameter with lengths between 0.5 and 10 micrometres.
- Montmorillonite intermixes
Mesoporous material (2–50 nm)
Macroporous material (>50 nm)
Molecular sieves are often utilized in the petroleum industry, especially for drying gas streams. For example, in the liquid natural gas (LNG) industry, the water content of the gas needs to be reduced to less than 1 ppmv to prevent blockages caused by ice.
Under the term zeolites, molecular sieves are used for a wide range of catalytic applications. They catalyze isomerisation, alkylation, and epoxidation, and are used in large scale industrial processes, including hydrocracking and fluid catalytic cracking.
They are also used in the filtration of air supplies for breathing apparatus, for example those used by scuba divers and firefighters. In such applications, air is supplied by an air compressor and is passed through a cartridge filter which, depending on the application, is filled with molecular sieve and/or activated carbon, finally being used to charge breathing air tanks. Such filtration can remove particulates and compressor exhaust products from the breathing air supply.
The U.S. FDA has as of April 1, 2012 approved sodium aluminosilicate for direct contact with consumable items under 21 CFR 182.2727. Prior to this approval Europe had used molecular sieves with pharmaceuticals and independent testing suggested that molecular sieves meet all government requirements but the industry had been unwilling to fund the expensive testing required for government approval.
Methods for regeneration of molecular sieves include pressure change (as in oxygen concentrators), heating and purging with a carrier gas (as when used in ethanol dehydration), or heating under high vacuum. Regeneration temperatures range from 175 °C to 315 °C depending on molecular sieve type. In contrast, silica gel can be regenerated by heating it in a regular oven to 120 °C (250 °F) for two hours. However, some types of silica gel will "pop" when exposed to enough water. This is caused by breakage of the silica spheres when contacting the water.
|Model||Pore diameter (Ångström)||Bulk density (g/ml)||Adsorbed water (% w/w)||Attrition or abrasion, W (% w/w)||Usage|
|3Å||3||0.60–0.68||19–20||0.3–0.6||Desiccation of petroleum cracking gas and alkenes, selective adsorption of H2O in insulated glass (IG) and polyurethane|
|4Å||4||0.60–0.65||20–21||0.3–0.6||Adsorption of water in sodium aluminosilicate which is FDA approved (see below) used as molecular sieve in medical containers to keep contents dry and as food additive having E-number E-554 (anti-caking agent); Preferred for static dehydration in closed liquid or gas systems, e.g., in packaging of drugs, electric components and perishable chemicals; water scavenging in printing and plastics systems and drying saturated hydrocarbon streams. Adsorbed species include SO2, CO2, H2S, C2H4, C2H6, and C3H6. Generally considered a universal drying agent in polar and nonpolar media; separation of natural gas and alkenes, adsorption of water in non-nitrogen sensitive polyurethane|
|5Å-DW||5||0.45–0.50||21–22||0.3–0.6||Degreasing and pour point depression of aviation kerosene and diesel, and alkenes separation|
|5Å small oxygen-enriched||5||0.4–0.8||≥23||Specially designed for medical or healthy oxygen generator|
|5Å||5||0.60–0.65||20–21||0.3–0.5||Desiccation and purification of air; dehydration and desulphurization of natural gas and liquid petroleum gas; oxygen and hydrogen production by pressure swing adsorption process|
|10X||8||0.50–0.60||23–24||0.3–0.6||High-efficient sorption, be used in desiccation, decarburization, desulphurization of gas and liquids and separation of aromatic hydrocarbon|
|13X||10||0.55–0.65||23–24||0.3–0.5||Desiccation, desulphurization and purification of petroleum gas and natural gas|
|13X-AS||10||0.55–0.65||23–24||0.3–0.5||Decarburization and desiccation in the air separation industry, separation of nitrogen from oxygen in oxygen concentrators|
|Cu-13X||10||0.50–0.60||23–24||0.3–0.5||Sweetening (removal of thiols) of aviation fuel and corresponding liquid hydrocarbons|
- Approximate chemical formula: 2/3K2O•1/3Na2O•Al2O3• 2 SiO2 • 9/2 H2O
- Silica-alumina ratio: SiO2/ Al2O3≈2
3Å molecular sieves do not adsorb molecules whose diameters are larger than 3 Å. The characteristics of these molecular sieves include fast adsorption speed, frequent regeneration ability, good crushing resistance and pollution resistance. These features can improve both the efficiency and lifetime of the sieve. 3Å molecular sieves are the necessary desiccant in petroleum and chemical industries for refining oil, polymerization, and chemical gas-liquid depth drying.
3Å molecular sieves are used to dry a range of materials, such as ethanol, air, refrigerants, natural gas and unsaturated hydrocarbons. The latter include cracking gas, acetylene, ethylene, propylene and butadiene.
3Å molecular sieve is utilized to remove water from ethanol, which can later be used directly as a bio-fuel or indirectly to produce various products such as chemicals, foods, pharmaceuticals, and more. Since normal distillation cannot remove all the water (an undesirable byproduct from ethanol production) from ethanol process streams due to the formation of an azeotrope at around 95 percent concentration, molecular sieve beads are used to separate ethanol and water on a molecular level by adsorbing the water into the beads and allowing the ethanol to pass freely. Once the beads are full of water, temperature or pressure can be manipulated, allowing the water to be released from the molecular sieve beads.
3Å molecular sieves are stored at room temperature, with a relative humidity not more than 90%. They are sealed under reduced pressure, being kept away from water, acids and alkalis.
- Chemical formula: Na2O•Al2O3•2SiO2•9/2H2O
- Silica-alumina ratio: SiO2/ Al2O3≈2
4Å molecular sieves are widely used to dry laboratory solvents. They can absorb water and other molecules with a critical diameter less than 4 Å such as NH3, H2S, SO2, CO2, C2H5OH, C2H6, and C2H4. It is widely used in the drying, refining and purification of liquids and gases (such as the preparation of argon).
Polyester agent additives
These molecular sieves are used to assist detergents as they can produce demineralized water through calcium ion exchange, remove and prevent the deposition of dirt. They are widely used to replace phosphorus. The 4Å molecular sieve plays a major role to replace sodium tripolyphosphate as detergent auxiliary in order to mitigate the environmental impact of the detergent. It also can be used as a soap forming agent and in toothpaste.
Harmful waste treatment
4Å molecular sieves can purify sewage of cationic species such as ammonium ions, Pb2+, Cu2+, Zn2+ and Cd2+. Due to the high selectivity for NH4+ they have been successfully applied in the field to combat eutrophication and other effects in waterways due to excessive ammonium ions. 4Å molecular sieves have also been used to remove heavy metal ions present in water due to industrial activities.
- The metallurgical industry - separating agent, separation, extraction of brine potassium, rubidium, cesium, etc.
- Petrochemical industry, catalyst, desiccant, adsorbent
- Agriculture - soil conditioner;
- Medicine - load silver zeolite antibacterial agent.
- Chemical formula: 0.7CaO•0.30Na2O•Al2O3•2.0SiO2 •4.5H2O
- Silica-alumina ratio: SiO2/ Al2O3≈2
5Å molecular sieves are often utilized in the petroleum industry, especially for the purification of gas streams and in the chemistry laboratory for separating compounds and drying reaction starting materials. They contain tiny pores of a precise and uniform size, and are mainly used as an adsorbent for gases and liquids.
5Å molecular sieves are used to dry natural gas, along with performing desulfurization and decarbonation of the gas. They can also be used to separate mixtures of oxygen, nitrogen and hydrogen, and oil-wax n-hydrocarbons from branched and polycyclic hydrocarbons.
5Å molecular sieves are stored at room temperature, with a relative humidity less than 90% in cardboard barrels or carton packaging. The molecular sieves should not be directly exposed to the air and water, acids and alkalis should be avoided.
- "Molecular Sieve Definition - Definition of Molecular Sieve - What Is a Molecular Sieve?". Chemistry.about.com. 2013-12-18. Retrieved 2014-02-26.
- J. Rouquerol; et al. (1994). "Recommendations for the characterization of porous solids (Technical Report)" (free download pdf). Pure & Appl. Chem. 66 (8): 1739–1758. doi:10.1351/pac199466081739.
- "COATED MOLECULAR SIEVE - Patent application". Faqs.org. 2010-03-18. Retrieved 2014-02-26.
- Brindley, George W. (1952). "Structural mineralogy of clays". Clays and Clay Minerals. 1: 33–43. Bibcode:1952CCM.....1...33B. doi:10.1346/CCMN.1952.0010105.
- "Desiccant Types". SorbentSystems.com. Retrieved 2014-02-26.
- Mann, B. F.; Mann, A. K. P.; Skrabalak, S. E.; Novotny, M. V. (2013). "Sub 2-μm Macroporous Silica Particles Derivatized for Enhanced Lectin Affinity Enrichment of Glycoproteins". Analytical Chemistry. 85 (3): 1905–1912. PMC . PMID 23278114. doi:10.1021/ac303274w.
- Williams, D. B. G., Lawton, M., "Drying of Organic Solvents: Quantitative Evaluation of the Efficiency of Several Desiccants", The Journal of Organic Chemistry 2010, vol. 75, 8351. doi: 10.1021/jo101589h
- Pujadó, P. R.; Rabó, J. A.; Antos, G. J.; Gembicki, S. A. (1992-03-11). "Industrial catalytic applications of molecular sieves". Catalysis Today. 13 (1): 113–141. doi:10.1016/0920-5861(92)80191-O.
-  Archived April 16, 2012, at the Wayback Machine.
- "Sec. 182.2727 Sodium aluminosilicate.". U.S. Food and Drug Administration. 1 April 2012. Retrieved 10 December 2012.
- "Molecular Sieve Desiccant". DesiccantPacks.net. Retrieved 2014-02-26.
- "Molecular Sieves". Sigma-Aldrich. Retrieved 2014-02-26.
- Spence Konde, "Preparation of High-Silica Zeolite Beads From Silica Gel," retrieved 2011-09-26
- "Molecular Sieve,yiyuan Molecular Sieves". Chemicalpackingcorp.com. Retrieved 2014-02-26.
- "Hengye Inc.". Hengye Inc. Hengye Inc. Retrieved Hengye Inc. June 2015. Check date values in:
- Williams, D. B. G.; Lawton, M., "Drying of Organic Solvents: Quantitative Evaluation of the Efficiency of Several Desiccants", The Journal of Organic Chemistry 2010, 75, 8351-8354. doi:10.1021/jo101589h